Author
others
View
7
Download
0
Embed Size (px)
2.c.iv.
Metastable Austenitic Stainless Steels and the Effect of Deformation-Induced Phase Transformation on the Fatigue Properties Hans-J. Christ, Andrei Grigorescu, Carsten Müller-Bollenhagen, Martina Zimmermann
1. Sheet forming of austenitic stainless steels Austenitic stainless steels cover about three quarters of the world production of non-corroding steels and are the mostly used stainless steels in sheet metal forming. They are characterized by a low yield stress, high ductility, strong cold work hardening and excellent corrosion resistance. The good corrosion properties result from high Cr contents. However, since Cr stabilizes the ferritic phase and the austenitic condition is more favourable in terms of the mechanical properties, other elements have to be added which support the austenite formation. The most important alloy in this respect is Ni in austenitic stainless steels. As can be seen in Fig. 1 a minimum of the Ni content for the stabilization of austenite exists at about 18 wt.% Cr. Higher Cr contents prohibit the formation of martensite, however the formation of δ ferrite is promoted, which itself must be prevented by a higher concentration of Ni. Since a high Ni content is connected to high costs, most of the common CrNi steels contain 18 wt.% Cr and 8 wt.% Ni.
Fig. 1: Effect of nickel and chromium on the microstructural condition of 0.1 wt. % C steel (after Schumann
1990)
Besides Cr and Ni numerous other alloying elements are used in austenitic stainless steels, which either stabilize the ferritic phase (e.g., Mo, Ti, Nb, V) or the austenitic phase (in particular C, N, Mn). For the sake of a simple assessment of the phase composition by means of empirical equations, a Cr equivalent and a Ni equivalent are calculated from the concentrations of all ferrite-stabilizing and austenite-stabilizing elements, respectively. A survey of all available equations suitable to calculate the equivalent values and the corresponding Schaeffler diagrams showing the approximate phase compositions can be found in Schoss (2001). The variation in the
concentrations of the alloying elements allows for a selective adjustment of the phase composition and the metastability of austenite.
2. Martensitic transformation in CrNi steels Originally, the term martensitic transformation was used exclusively in the context of steels. Today, this term is generally applied to diffusionless phase transformations in various materials (e.g., in shape memory alloys). Austenite denotes the high-temperature phase, while martensite refers to the low-temperature phase (Hosford 2005). The martensitic transformation can take place thermally induced, stress-induced and strain-induced. Olson and Cohen (1975) stated that stress-induced martensite formation occurs at such nucleation sites, where also thermally induced martensite is triggered, though the thermodynamic effect is supported by the external stress. In the case of deformation-induced martensite, however, new nucleation sites are formed by plastic deformation. Figure 2 summarizes the possibilities of the martensite formation as a function of temperature and defines characteristic temperatures of martensite formation. Below the Md temperature deformation-induced martensite can form, if the stress reaches the required level. Between Ms and Ms,σ a martensite formation is possible as a consequence of elastic deformation (stress-induced) and below Ms thermally induced martensite is possible. From the point of view of sheet forming, certainly the deformation-induced martensite formation is most important. In this context the austenitic phase is called “metastable“, if a deformation at room temperature can lead to a transformation into martensite.
Fig. 2: Different ways of martensite formation in metastable austenitic steels (after Olson and
Cohen 1972)
In metastable austenitic stainless steels the deformation-induced transformation of the γ phase (austenite) can lead to α′ martensite (bcc) and/or to ε martensite (hcp). For the mechanical properties the α′ martensite is more important, because α′ has a higher strength than the austenitic phase at identical chemical composition. During the γ→α′ transition a volume expansion takes place, which is reported to be between 2 % and 5 % in the literature (Angel 1954, Nishiyama 1978, Bowe et al. 1988, Suresh 1998) and depends strongly on the carbon content. The ε martensite has a very similar specific volume as the austenitic phase, and the mechanical properties are
controversially discussed in the literature. Nevertheless, it seems to be commonly accepted that the ε phase posseses a lower strength than the α′ phase.
3. Formation of martensite nucleation sites Many studies performed during the last decades document that the α′ martensite preferentially forms at shear bands and points of intersection of shear bands (Venables 1962, Mangonon and Thomas 1970, Staudhammer et al. 1983, Bracke et al. 2007). Figure 3 depicts the α′ martensite formation in an austenitic steel at intersections of shear bands in a TEM micrograph. Based on the concept of Bogers and Burgers (1964), Olson and Cohen (1972) could show that these intersections provide energetically favourable conditions for the formation of α′ martensite. In their model, a shear band with a stacking fault on every other plain (corresponding to the lattice structure of ε martensite) intersects with a shear band on every third plain (distorted ε martensite). At the point of intersection of these two shear bands the correct stacking sequence of α′ martensite is present (Fig. 4). A recent molecular dynamic simulation confirms this theory (Sinclair and Hoagland 2008). The critical width of a shear band for martensite formation lies at 50-70 Å according to a TEM study of Staudhammer et al. (1983). This corresponds to a minimum of about 24 stacked atomic layers.
With regard to the exact position and properties of the martensite nucleation sites, very different experimental observations are reported in the literature. Some authors find α′ martensite exclusively at intersections of ε martensite (Mangonon and Thomas 1970), others in turn find α′ martensite at points of intersection of shear bands or at single shear bands (Spencer et al. 2009a, Arpan Das et al. 2008, Lee and Lin 2000). Furthermore, martensite formation at grain boundary triple points was observed (Arpan Das et al. 2008). Obviously, different forming conditions lead to different preferred martensite nucleation sites and different transformation paths.
Fig. 3: TEM micrograph showing α′ martensite formation at points of intersection of shear bands (Spencer et al. 2004)
Fig. 4: Shear bands in a hard sphere model. One shear band consists of ε martensite, the second contains stacking faults at every third plain (from Sinclair and Hoagland 2008).
α′
In this context, the value of the stacking fault energy γSF seems to play a significant role. It is commonly accepted that the tendency of austenitic steels to form deformation-induced martensite depends on the stacking fault energy (Schuman 1975, Olson and Cohen 1975). A low stacking fault energy promotes the formation of planar lattice defects such as stacking faults, deformation twins or ε martensite. Since these defects serve as nucleation sites for the formation of α′ martensite, there is a direct connection between the value of γSF and the tendency of deformation-induced martensite formation. In summary, it can be stated that the different results reported in the literature regarding the nucleation site of martensite are mainly a consequence of differences in γSF of the material study, in the forming temperature and/or forming rate. A clear dominance of α′ martensite formation at shear band intersections exists for high fractions of deformation-induced martensite.
4. Factors affecting the martensite formation The formation of martensite during a forming process applied to an austenitic stainless steel depends strongly on the chemical composition, the temperature, the strain, the strain rate and the stress state. Some of these influences are briefly described in the following. As mentioned before, the stability of the austenitic phase, i.e., the tendency to form deformation-induced martensite, is affected by the value of the stacking fault energy, which itself is determined by the chemical composition. This is often expressed by empirical equations which connect the Md30 temperature with the concentrations of alloying elements. The Md30 temperature is the temperature at which a deformation of 30 % leads to a martensite content of 50 vol.%. If this temperature lies below room temperature, martensite is not formed in a forming process without cooling. Nohara et al. (1977) proposed that the Md30 temperature of CrNi steels can be described by the following equation: Md30
GS is the ASTM grain size number. Equation 1 indicates that interstitially dissolved elements, such as C and N, are particularly strong austenite stabilizers. Small variations in the chemical composition within a sample/part (segregation) can lead to an inhomogeneous martensite distribution (Lichtenfeld et al. 2006).
(°C)=551-462·(C+N)-9.2·Si-8.1·Mn-13.7·Cr-29·(Ni+Cu)-18.5·Mo-68·Nb-1.42·(GS-8) (1)
A reduction of the temperature increases the thermodynamic driving force of the martensite formation and, hence, leads to a higher martensite formation rate during forming. Moreover, a temperature decrease lowers the stacking fault energy supporting also an augmented martensite formation. Austenitic steels are known for a low thermal conductivity and a high self-heating as a consequence of the dissipative energy of deformation. Therefore, during forming a temperature increase may result strongly affecting the martensite formation. The increase in the number of martensite nuclei depends on the stress and strain state. Murr et al. (1982) showed by means of TEM examinations of uniaxially and biaxially deformed specimens that the formation rate of shear band intersections is significantly higher under biaxial load. The martensite formation in torsion lies between that of uniaxial tension and biaxial tension (Frehn 2004). In compression tests, mostly less martensite was found as compared to tensile tests (Patel and Cohen 1953, Powell 1958, Frehn 2004). This can basically be attributed to the volume expansion which accompanies the austenite→martensite transformation.
In order to understand the effect of strain rate on the martensite formation two aspects have to be distinguished: the direct strain rate effect and the indirect one, which results from the increasing self-heating during deformation with increasing strain rate. The second effect simply is a consequence of the fact that at higher deformation rate the time per strain increment available for heat “leakage” is smaller. Consequently, samples are heating up and the thermodynamic driving force of the martensite formation is reduced (De et al. 2006, Santacreu et al. 2006, Lichtenfeld et al. 2006). A completely separate consideration of both strain rate effects is not possible. However, some studies indicate that high strain rates lead to enhanced martensite formation at constant temperature (Hecker et al. 1982, Lee and Lin 2000, De et al. 2006). An increase of the strain rate manifests itself at first in a more pronounced formation of stacking faults and shear bands (Talonen et al. 2005) and subsequently in the formation of ε martensite and twins (Ferreira et al. 2004).
5. Modelling approaches for martensite formation The simulation of the forming process and the purposeful control of the martensite formation by means of the forming parameters require a martensite formation model that takes the factors discussed above, such as strain, chemical composition, temperature, and deformation rate, into account. Because of the sensibility to changes in the chemical composition, there is always the need to adapt the martensite formation model to the specific heat of the material considered. Newly proposed models describe the martensite formation mostly in an incremental form as dVM/dε, i.e., the differential change of the martensite volume VM with strain ε. This allows a simulation of the forming process even if the forming temperature and the stress state changes. Many recent approaches to model the martensite formation are based on the assumptions and observations of Olson and Cohen (1975) and of Tsuta and Cortés (1993). The model of Olson and Cohen (1975) assumes that the formation of martensite embryos is directly depending on the number of shear band intersections. Shear bands is used here as a general term comprising ε martensite, superimposed stacking faults and deformation twins. The number of shear band intersections is determined from the shear band volume VSB. The shear band volume is calculated from the plastic strain assuming a decreasing shear band formation rate dVSB/dε with increasing shear band volume VSB.
(2)
The constant α determines the shear band formation rate and depends on the stacking fault energy and the strain rate.
If a shear band has an average volume SBv , the number of shear bands per austenite volume unit SB
VN is
SBSBSB
V vVN /= . (3)
Olson and Cohen assume that the number of shear band intersections XVN per
volume unit depends on the number of shear bands SBVN in the following form
nSBV
XV NKN )(= . (4)
( )SBSB V
ddV
−⋅= 1αε
K denotes a constant that depends on the grain size. The incremental increase of the number of martensite embryos M
VdN is determined by the increase of the shear band intersections, which transform into a martensite embryo with a probability of p
XV
MV dNpdN = . (5)
If it is now assumed that the average volume of a martensite embryo Mv is independent of the martensite fraction, then the increase of martensite per austenite volume can be calculated from the martensite embryo volume Mv and the change of the number of embryos M
VdN
MVM
M
M dNvV
dV⋅=
−1. (6)
Inserting Eqs. 1-5 into Eq. 6 and integrating the resulting equation leads to
})]exp(1[exp{1 nMV εαβ ⋅−−−−= (7)
pv
Kvn
SB
M
)(=β . (8)
The original formulation of the model of Olson and Cohen is not suitable for the simulation of non-isothermal forming processes, because α and β are considered to be constant during the process. Therefore, the model was further developed by a number of authors (Hecker et al. 1982, Stringfellow et al. 1992, Han et al. 2004 and Han et al. 2008). The advancement of the Olson and Cohen model by Tomita and Iwamoto (1995), called TI model in the following, found high acceptance. They took experimental results into account which documented an influence of the strain rate on the formation of shear bands. As a consequence the effect of strain rate and temperature on the Olson&Cohen parameters α (see Eq. 2) was formulated as
m
r
aTT
⋅++=εεαααα
)( 32
21 . (9)
Here 321 ,, ααα are constants, rε is a reference strain rate, aε is the strain rate in austenite, m is a strain rate sensitivity exponent and T is the temperature. The approach after Stringfellow et al. (1992) was used in a simplified form in order to calculate the martensite formation probability and, hence, the Olson&Cohen parameter β. For this purpose a Gaussian normal distribution was applied in the following form
'2
)'(exp2 2
20 dgggp
g
g∫∞−
−−=⋅=
σπηηβ (10)
Σ+−= 1gTg . (11)
Here η is a geometrical constant, g is the normalized thermodynamic driving force, g0 and σg are the mean value and the standard deviation of the probability distribution, respectively, g1 is a constant and Σ=σii/3 is the triaxiality parameter. The TI model has been implemented in FE simulations by various authors (e.g., Garion et al. 2005, Hedström et al. 2009) and it has been applied to TRIP steels (Dan et al. 2007). The second elementary model, which has already been mentioned before and which is used for current research activities, is the model of Tsuta and Cortés (1993). The basic assumption consists of a linear correlation between the martensite formation rate dVM/dε related to the present austenite volume fraction VA and the formed martensite per strain VM/ε. The models of Hänsel (1998) and Springub (2006) are both incrementally formulated modifications of the model of Tsuta and Cortés (1993) and are also of phenomenological nature.
6. Effect of martensite on the mechanical properties of austenitic stainless steels
Already in 1954, Angel (1954) found in tensile tests on different austenitic stainless steels an unexpected increase of the flow stress which changes proportional to the content of martensite. The reason for the stress increase was identified as the higher strength of the martensitic phase. The positive effect of the γ→α′ phase transformation on the mechanical properties was subject of many investigations in the last decades and is often called TRIP effect (TRansformation-Induced Plasticity). The term TRIP comprises the numerous effects of the α′ martensite formation on the mechanical properties of martensitically transforming steels, which result from the increase of both ductility and flow stress (e.g., Lichtenfeld et al. 2006), the higher strength of the martensitic phase and the intrinsic shape change of the martensitic transformation (shear and volume change, e.g., Han et al. 2004). The TRIP effect causes a pronounced ductility increase. The larger fracture strain is commonly explained as a consequence of a local martensite formation at sites of high plastic deformation impeding necking and retarding fracture (Huang et al 1989). The simplest way of an analytical description of the deformation behaviour of metastable austenitic stainless steels is to develop a modification of one of the classical empirical equations used for the stress-strain relationship. Often the contributions of austenite and α′ martensite are simply combined in a summation. The effect of ε martensite on the mechanical properties is mostly neglected. For example, Hänsel (1998) uses the approach after Hockett-Sherby for the description of the flow curve of a phase mixture. It is assumed that the strength of martensite leads to a constant strength increase 'αγσ →∆ in the moment of the transformation. An additive treatment of the strength contributions leads to
MMtot VVV ⋅∆+⋅+⋅= → 'αγγγγ σσσσ (12)
or simplified
Mtot V⋅∆+= → 'αγγ σσσ . (13)
Here, γσ denotes the flow stress of the γ phase, totσ means the flow stress of the phase mixture, and Vγ and VM are the volume fractions of the γ and the α′ phase, respectively.
The use of the Hockett-Sherby hardening law yields the following equation
m
Mq
HSHSHStotw VeABB
n
⋅⋅∆+⋅−−= →
−
0' )])(([
εεσσ αγ
ε
. (14)
AHS, BHS, m, n, q and 'αγσ →∆ are constants which need to be adapted to the experimental data. Tomita and Iwamoto (1995) calculate the flow stresses separately for both phases according to
])exp(1[(exp( 3
54 21
γ
γγγγγ
γ εσ CCCTCC −−+−= (15)
])exp(1[(exp( 3
54 21
α
ααααα
α εσ CCCTCC −−+−= . (16)
Equations 15 and 16 contain ten constants αγ ,5...1=iC , which do not have a direct physical
meaning and must be fitted to the experimental data. By means of an energy criterion these equations are nonlinearly coupled for the calculation of the flow stress of the phase mixture. Similar approaches are reported by Onyuna et al. (2004) or Sangal et al. (1985). More satisfactory from a physical point of view are approaches which calculate the mechanical behaviour of metastable austenitic stainless steels by means of the microstructural changes occurring during deformation (e.g., changes of the dislocation density, grain size, ...). The foundation of these models is the classical relation between dislocation density and flow stress
ρασσ γγ MGbMK+= 0 . (17)
σγ0 denotes the friction stress of the austenite, M is the Taylor orientation factor, G denotes the shear modulus, b is the Burgers vector, ρ is the dislocation density and αMK is a constant (≈0.4 for austenitic steels after Bouquerel et al. (2006)). The change in the dislocation density resulting from plastic deformation dρ/dε can be described after Mecking and Kocks (1981) by the combination of a dislocation formation rate and a dislocation annihilation rate (dynamic recovery) according to
ρερ f
bMdd
−Λ
=1
. (18)
Λ denotes the mean free dislocation path and f is a constant. Perlade et al. (2003) use the model concept of Mecking and Kocks and assume furthermore that the mean free dislocation path is limited by the spacing of the martensite plates (see Fig. 5).
Fig. 5: Limitation of the mean free dislocation path Λ by the formation of martensite in the model of Perlade et al. (2003). The reduction of Λ through other dislocations is not shown.
If several obstacles (grain boundaries, martensite needles, dislocations) impede the dislocation motion, the following expression can be used after Perlade et al. (following Estrin and Mecking 1984):
(19)
λ is the mean martensite plate spacing, dγ is the austenite grain size and k is a constant. For practical purposes it is important to note that the mean spacing of the martensite plates can be deduced from metallographic data, i.e., the mean width of the martensite plates c and the martensite content VM.
M
M
VVc −
=12λ (20)
The parameters f (Eq. 18) and k (Eq. 19) are unknown and must be adapted to the experimental data. A similar approach, also based on the model of Mecking and Kocks, was developed by Bouquerel et al. (2006). They assume that the grain size dγ in Eq. 19 is a function of the martensite content VM.. The term for the mean martensite plate spacing λ is omitted and the following equation results
ρρερ
γ
fkVdbMd
d
M
−
+
−=
3 111 . (21)
The strengthening of the martensitic phase ∆σα= σα-σα0 is calculated using the equation
M
MK LfMfbGM
α
αααα
εασσσ )exp(10
−−=∆=− . (22)
σα0 is the yield strength of the martensite, LM is the width of the martensite plates, and fα is a constant.
∑Λ
=Λ i
11 ρ+λ
+=Λ γ
k1d11
The macroscopic flow stress of the phase mixture is calculated in the model of Bouquerel et al. (2006) by applying the following role of mixture
'' )())(1( nM
nMtot VV αγ σσσ +−= . (23)
The exponent n′ must be fitted to experimental data as it is also the case for the parameters f, k and fα. Both last mentioned approaches (Bouquerel 2006 et al. and Perlade et al. 2003) enable a microstructural-based assessment of the mechanical properties at a rather small number of model parameters as compared to the solely empirical models. Moreover, the computational capacity needed is small so that these models are suitable for an online control of a forming process.
7. Fatigue behaviour in the transition regime from high to very-high number of cycles to failure
The engineering term “fatigue limit” describes the stress amplitude, which can be endured infinitely often by a material without leading to failure. Since many newer results indicate that failure can also occur after very high number of loading cycles, it appears very doubtful if a true fatigue limit exists (Mughrabi 2010). Therefore it seems to be more appropriate to distinguish between a HCF (High Cycle Fatigue) fatigue strength which is connected to an ultimate number of loading cycles Nult mostly defined on the basis of the available test frequency in combination with the acceptable time per fatigue test and the VHCF (Very High Cycle Fatigue) fatigue strength which defines the stress amplitude below which no failure occurs, if a Nult in the order of 109 is applied. The term VHCF fatigue limit should only be used if in the VHCF regime a horizontal course of the S-N curve actually exists. The stress amplitude of the HCF fatigue strength corresponds for most of the metallic materials to a plastic strain amplitude between 10-5 and 10-4 (Klesnil and Lukás 1992). Cyclic loading in the VHCF regime is assumed to cause only very localized plastic deformation and a global plastic deformation can hardly be monitored (Berger and Christ 2011). An interpretation of the HCF and VHCF fatigue strength from a microstructural point of view is that though at these stress amplitudes fatigue cracks can initiate and these cracks can grow as microstructurally short cracks, they are stopped by microstructural obstacles before they can reach a critical length. For the HCF fatigue strength this critical length lies in the order of the grain size.
8. Effect of martensite on the fatigue behaviour of austenitic stainless steels
The martensite formation under cyclic loading is similar to monotonic conditions and depends strongly on the specimen temperature, the plastic strain amplitude and the number of loading cycles (Krupp et al. 2008, Smaga et al. 2008). Often a threshold value of the plastic strain amplitude in the order of 3·10-3 is reported, above which martensite can form (Kaleta and Zicetek 1997, Bayerlein et al. 1989). This threshold value seems to depend very sensibly on the chemical composition (i.e., austenite stability). At identical cumulative plastic strains higher strain amplitudes lead to stronger martensite formation, for which reason Smaga et al. (2008) propose the use of the cumulative energy density as a reference parameter for the modelling of the martensite formation under cyclic loading conditions. Further model approaches are described by Nebel (2002). The α′ martensite which is formed in fatigue tests is often
inhomogeneously distributed across the specimen cross-section. Stronger martensite formation is reported for the surface (Maier et al. 1993, Kalkhof et al. 2004) as well as for the centre of the sample (Kalkhof et al. 2004, Nebel 2002). The effect of martensite formation on the fatigue behaviour can roughly be attributed to three mechanisms. The first mechanism is the effect of the martensite content on the cyclic stress-strain response. Many authors have shown that the martensitic transformation changes the cyclic deformation behaviour drastically. The high strength of the martensitic phase leads to a cyclic hardening and a reduction of ductility (Maier et al. 1993, De Backer et al. 2001, Nikitin and Besel 2008, Smaga et al. 2008). The volume expansion which accompanies the γ→ α′ transformation leads to the development of a negative mean stress in total-strain-controlled and plastic-strain-controlled fatigue tests (Maier et al. 1993, Glage et al. 2009). The second mechanism concerns the local martensite formation. Pineau and Pelloux (1974) could show that the local formation of martensite in the plastic zone ahead of the tip of a fatigue crack retards the crack propagation. The reason for this phenomenon is most probably the compressive stresses, which result from the martensitic transformation, reducing the effective stress intensity factor. This mechanism has been confirmed in many studies (see Bowe et al. 1988, Suresh 1998) and is called ”transformation-induced crack closure” in textbooks. If the martensite formation occurs not only locally at the crack tip, but takes place globally in the sample leading to a high martensite fraction, then the crack can grow through the martensite and the propagation rate is higher as compared to the one in austenite (Bowe et al. 1988, Pineau and Pelloux 1974). The third mechanism is the direct influence of an established two-phase microstructure on the fatigue crack propagation behaviour. Though this aspect has not been considered systematically in the literature for metastable austenitic stainless steels, investigations have been carried out on duplex stainless steels (Düber 2007). It was clearly shown that both the growth mechanisms and the growth rate of microstructurally short fatigue cracks changes with the phase surrounding the crack tip. The effect of martensite on the VHCF properties of austenitic stainless steels will be considered in detail in chapter 4b. Since VHCF loading should lead to only local plastic deformation, a significant change in the martensite content is not to be expected in the VHCF regime. Hence, the deformation-induced martensite results mainly from a predeformation (e.g., introduced during sheet forming). In general, an optimum of the VHCF strength can be expected for a certain martensite content, because of the conflictive effect of the increase of strength on the one hand and notch sensitivity on the other hand.
References Angel T. (1954): Formation of Martensite in Austenitic Stainless Steel, J. Iron and Steel Inst.:
JISI, 177, 165-174.
Arpan Das; Sivaprasad, S.; Ghosh, M.; Chakraborti, P.C.; Tarafder, S. (2008): Morphologies and Characteristics of Deformation Induced Martensite during Tensile Deformation of 304 LN Stainless Steel, Mater. Sci. Eng. A, 486, 283-286.
Bayerlein, M.; Christ, H.-J.; Mughrabi, H. (1989): Plasticity-Induced Martensitic Transformation during Cyclic Deformation of AISI 304L Stainless Steel, Mater. Sci. Eng. A, 114, 11-16.
Berger C.; Christ H.-J. (2011): Proceedings VHCF5, Fifth International Conference on Very High Cycle Fatigue, 28.-30. Juni 2011, Berlin, DVM, Berlin, 2011
Bogers, A.J.; Burgers, W.G. (1964): Partial Dislocations on the {110} Planes in the B.C.C. Lattice and the Transition of the F.C.C. into the B.C.C. Lattice, Acta Metall., 12, 255-261.
Bouquerel, J.; Verbeken, K.; De Cooman, B.C. (2006): Microstructure-Based Model for the Static Mechanical Behaviour of Multiphase Steels, Acta Mater., 54, 1443-1456.
Bowe, K. H.; Hammerschmidt, E.; Hornbogen, E.; Hühner, M. (1988): Bruchmechanische Eigenschaften von metastabilen Austeniten, Materialwiss. Werkstofftech., 19, 193-201.
Bracke, L.; Kestens, L.; Penninga, J. (2007): Transformation Mechanism of α′-Martensite in an Austenitic Fe–Mn–C–N Alloy, Scr. Mater., 57, 385-388.
Dan, X.J.; Zhang, W.G.; Li, S.H.; Lin, Z.Q. (2007): A Model for Strain-Induced Martensitic Transformation of TRIP-Steel with Strain, Comput. Mater. Sci., 40, 101-107.
De Backer, F.; Schoss, V.; Maussner, G. (2001): Investigations on the Evaluation of the Residual Fatigue Life-Time in Austenitic Stainless Steels, Nucl. Eng. Des., 206, 201-219.
De, A.K.; Speer, J.G.; Matlock, D.K.; Murdock, D.C.; Mataya, M.C.; Comstock, Jr., R.J. (2006): Deformation-Induced Phase Transformation and Strain Hardening in Type 304 Austenitic Stainless Steel, Metall. Mater. Trans. A, 37, 1875-1885.
Düber, O. (2007): Untersuchungen zum Ausbreitungsverhalten mikrostrukturell kurzer Ermüdungsrisse in zweiphasigen metallischen Werkstoffen am Beispiel eines austenitisch-ferritischen Duplexstahls, Fortschritt-Berichte VDI, Reihe 5, Nr. 730, VDI-Verlag, Düsseldorf.
Estrin, Y.; Mecking, H. (1984): A Unified Phenomenological Description of Work Hardening and Creep Based on One-Parameter Models, Acta Metall., 32, 57-70.
Ferreira, P.J.; Vander Sande, J.B.; Amaral Fortes, M.; Kyröläinen, A. (2004): Microstructure Development during High-Velocity Deformation, Metall. Mater. Trans. A, 35, 3091-3101.
Frehn, A. (2004): Einfluss von Umformtemperatur und -geschwindigkeit auf das Umformvermögen von austenitischen nichtrostenden Stählen, Dissertation, RWTH Aachen.
Garion, C.; Skoczen, B.; Sgobba, S. (2005): Constitutive Modelling and Identification of Parameters of the Plastic Strain-Induced Martensitic Transformation in 316L Stainless Steel at Cryogenic Temperatures, Int. J. Plast., 22, 1234-1264.
Glage, A.; Weidner, A.; Richter, T.; Trubitz, P.; Biermann, H. (2009): Low Cycle Fatigue Behavior and Microstructure of a High Alloyed Metastable Austenitic Cast TRIP-Steel, in Proc. of ESOMAT, herausgegeben von Sittner, P.; Heller, L.; Paidar, V., DP Sciences (www.esomat.org), paper 05007, DOI:10.1051/esomat/200905007.
Han, H.N.; Lee, C.G.; Oh, C.-S.; Lee, T.-H.; Kim, S.-J. (2004): A Model for Deformation Behavior and Mechanically Induced Martensitic Transformation of Metastable Austenitic Steel, Acta Mater., 52, 5203-5214.
Han, H.N.; Lee, C.G.; Suh, D.-W.; Kim, S.-J. (2008): A Microstructure-Based Analysis for Transformation Induced Plasticity and Mechanically Induced Martensitic Transformation, Mater. Sci. Eng. A, 485, 224-233.
Hänsel, A. (1998): Nichtisothermes Werkstoffmodell für die FE-Simulation von Blechumformprozessen mit metastabilen austenitischen CrNi-Stählen, Dissertation, ETH Zürich.
Hecker, S.; Stout, K.; Staudhammer, K.; Smith, J. (1982): Effects of Strain State and Strain Rate on Deformation-induced Transformation in 304 Stainless Steel: Part 1. Magnetic Measurements and Mechanical Behavior, Metall. Trans. A, 13A, 619-626.
Hedström, P.; Lindgren, L.E.; Almer, J.; Lienert, U.; Bernier, J.; Terner, M.; Odén, M. (2009): Load Partitioning and Strain-Induced Martensite Formation during Tensile Loading of a Metastable Austenitic Stainless Steel, Metall. Mater. Trans. A, 40A, 1073-5623.
Hosford, W. F. (2005): Mechanical Behaviour of Materials, Cambridge University Press.
Huang, G. L.; Matlock, D. K.; Krauss G. (1989): Martensite Formation, Strain Rate Sensitivity and Deformation Behaviour of Type 304 Austenitic Steel Sheet, Metall. Trans., 20A, 1239-1247.
Kaleta, J.; Zicetek, G. (1997): Identification of Cyclic Softening and σ-ε Hysteresis in Austenitic Steel with Plasticity-Induced Martensitic Transformation, Mater. Sci. Eng. A, 234-236, 680-683.
Kalkhof, D.; Grosse, M.; Niffenegger, M.; Leber, H.J. (2004): Monitoring Fatigue Degradation in Austenitic Stainless Steels, Fatigue Fract. Eng. Mater. Struct., 27, 595-607.
Klesnil, M.; Lukás, P. (1992): Fatigue of Materials, 2nd revised edition, Elsevier, Amsterdam.
Krupp, U.; West, C.; Christ, H.-J. (2008): Deformation-Induced Martensite Formation dDuring Cyclic Deformation of Metastable Austenitic Steel: Influence of Temperature and Carbon Content. Mater. Sci. Eng. A, 481-482, 713-717.
Lee, W.-S.; Lin, C.-F. (2000): The Morphologies and Characteristics of Impact-Induced Martensite in 304L Stainless Steel, Scr. Mater., 43, 777-782.
Lichtenfeld, J.A.; Mataya, M.C.; van Tyne, C.J. (2006): Effect of Strain Rate on Stress-Strain Behavior of Alloy 309 and 304L Austenitic Stainless Steel, Metall. Mater. Trans. A, 37, 147-161.
Maier, H.J.; Donth, B.; Bayerlein, M.; Mughrabi, H.; Meier, B.; Kesten, M. (1993): Optimierte Festigungssteigerung eines metastabilen austenitischen Stahles durch wechselverformungsinduzierte Martensitumwandlung bei tiefen Temperaturen , Z. Metallkd., 84, 820-826.
Mangonon, P.L.; Thomas, G. (1970): The Martensite Phases in 304 Stainless Steel, Metall. Trans., 1, 1577-1586.
Mecking, H.; Kocks, U.F. (1981): Kinetics of Flow and Strain-Hardening, Acta Metall., 29, 1865-1875.
Mughrabi, H. (2010): Fatigue, an Everlasting Materials Problem - Still en Vogue, Procedia Eng., 2, 3-26.
Murr, L.E.; Staudhammer, K.P.; Hecker, S.S. (1982): Effects of Strain State and Strain Rate on Deformation-Induced Transformation in 304 Stainless Steel: Part II. Microstructural Study. Metall. Trans. A, 13, 627-635.
Nebel, T. (2002): Verformungsverhalten und Mikrostruktur zyklisch beanspruchter metastabiler austenitischer Stähle, Dissertation, Kaiserlautern.
Nikitin, I.; Besel, M. (2008): Effect of Low-Frequency on Fatigue Behaviour of Austenitic Steel AISI 304 at Room Temperature and 25°C, Int. J. Fatigue, 30, 2044-2049.
Nishiyama, Z. (1978): Martensitic transformation, Academic Press, New York.
Nohara, K.; Ono, Y.; Ohashi, N. (1977): Composition and Grain-Size Dependencies of Strain-Induced Martensitic Transformation in Metastable Austenitic Stainless Steels, J. Iron and Steel Inst. Jpn, 63, 212-222.
Olson, G.B.; Cohen, M. (1972): A Mechanism for the Strain-Induced Nucleation of Martensitic Transformations, J. Less-Common Met., 28, 107-118.
Olson, G.B.; Cohen, M. (1975): Kinetics of Strain-Induced Martensitic Nucleation, Metall. Trans A, 6A, 791-795.
Onyuna, M.; Oettel, H.; Martin, U.; Weiß, A. (2004): On the Deformation Behaviour and Martensitic Transformations of Metastable Austenitic Steels, Adv. Eng. Mater., 7, 529-535.
Patel, J. R.; Cohen, M. (1953): Criterion for the Action of Applied Stress in the Martensitic Transformation, Acta Metall., 1, 531-538.
Perlade, A.; Bouaziz, O.; Furnemont, Q. (2003): A Physically Based Model for TRIP-aided Carbon Steels Behaviour, Mater. Sci. Eng. A, 356, 145-152.
Pineau, A.G.; Pelloux R. M. (1974): Influence of Strain-Induced Martensitic Transformations on Fatigue Crack Growth Rates in Stainless Steels, Metall. Trans., 5, 1103-112.
Powell, G.W.; Marshall, E.R.; Backofen, W.A. (1958): Strain Hardening of Austenitic Stainless Steel, Trans. of the ASM, 50, 478-497.
Sangal, S.; Goel, N.C.; Tangri, K. (1985): A Theoretical Model for the Flow Behavior of Commercial Dual-Phase Steels Containing Metastable Retained Austenite: Part 2, Calculation of Flow Curves, Metall. Trans. A, 16A, 2023-2029.
Santacreu, P.-O.; Glez, J.-C.; Chinouilh, G.; Fröhlich, T. (2006): Behaviour Model of Austenitic Stainless Steels for Automotive Structural Parts, Steel Res. Int., 77, 686-691.
Schoss, V. (2001): Martensitische Umwandlung und Ermüdung austenitischer Edelstähle, Gefügeveränderungen und Möglichkeiten der Früherkennung von Ermüdungsschädigun-gen, Dissertation, TU Bergakademie Freiberg.
Schumann, H. (1975): Verformungsinduzierte Martensitbildung bei austenitischen Stählen, Krist. Tech., 10, 401-411.
Schumann, H. (1990): Metallographie, 13. Auflage, Deutscher Verlag für Grundstoffindustrie, Stuttgart.
Sinclair, C.W.; Hoagland, R.G. (2008): A Molecular Dynamics Study of the fcc→bcc Transformation at Fault Intersections, Acta Mater., 56, 4160-4171.
Smaga, M.; Walther, F.; Eifler, D. (2008): Deformation-Induced Martensitic Transformation in Metastable Austenitic Steels, Mater. Sci. Eng. A, 483-484, 394-397.
Spencer, K.; Embury, J.D.; Conlon, K.T.; Véron, M.; Bréchet, Y. (2004): Strengthening via the Formation of Strain-Induced Martensite in Stainless Steels. Mater. Sci. Eng. A, 387-389, 873-881.
Spencer, K.; Embury, J.D.; Veron,M.; Yu-Zhang, K. (2009a): The Strain Induced Martensite Transformation in Austenitic Stainless Steels - Part 1 - Influence of Temperature and Strain History, Mater. Sci. Technol., 25, 7-17.
Springub, B. (2006): Semi-analytische Betrachtung des Tiefziehens rotationssymmetrischer Bauteile unter Berücksichtigung der Martensitevolution, Dissertation, PZH-Verlag, Universität Hannover.
Staudhammer, K.P.; Murr, L.E.; Hecker, S.S. (1983): Nucleation and Evolution of Strain-Induced Martensitic (B.C.C.) Embryos and Substructure in Stainless Steel: A Transmission Electron Microscope Study, Acta Metall., 31, 267-274.
Stringfellow, R.G.; Parks, D.M.; Olson, G.B. (1992): A Constitutive Model for Transformation Plasticity Accompanying Strain-Induced Martensitic Transformations in Metastable Austenitic Stainless Steels, Acta Metall. Mater., 40, 1703-1716.
Suresh, S. (1998): Fatigue of Materials, Cambridge University Press.
Talonen, J.,; Nenonen, P.; Pape, G.; Hänninen, H. (2005): Effect of Strain Rate on the Strain-Induced γ→α′-Martensite Transformation and Mechanical Properties of Austenitic Stainless Steels, Metall. Mater. Trans. A, 36, 421-431.
Tomita, Y.; Iwamoto, T. (1995): Constitutive Modeling of TRIP Steel and Its Application to the Improvement of Mechanical Properties, Int. J. Mech. Sci., 37, 1295-1305.
Tsuta, T.; Cortés, J.A. (1993): Flow Stress and Phase Transformation Analyses in Austenitic Stainless Steel under Cold Working, Part 2: Incremental Theory under Multiaxial Stress State by the Finite-Element Method, JSME Int J., 36, 63-72.
Venables, J.A. (1962): The Martensite Transformation in Stainless Steel. Philos. Mag., 7, 35-44.